259 | P a g e
Laboratory Evaluation of Warm Mix Asphalt
Vinod D. Ninawe1
, Shashikant A. Deshmukh2 12
Civil Engineering, Sant Gadge Baba Amravati University, (India)
Over the last thirty years, road traffic has luxuriate significantly and loading is progressively getting
cruddy due to the introduction of newer and ancillary big- wheel trucks with heavier and wider bodies in
India. This study emphasizes on the mix design considerations. In this study, bituminous concrete grade-1
(BC-1) and Zycotherm additive on the warm mix asphalt paving mix is used to achieve sufficient stability,
durability and to satisfy requirements. It is about the effect of Zycotherm additives on the Marshall
Properties, Indirect tensile strength, Tensile strength ratio and retained stability test of warm mix asphalt. The
specification such as Bulk density, Volume of air voids, Voids in Mineral Aggregates, Voids Filled with
Bitumen, Stability and Flow, Indirect Tensile Strength, Tensile Strength Ratio and Retained Stability are
determined. It is taken up with the objectives of to know the effect of Zycotherm on the properties of bituminous
mix. The different percentage of Zycotherm additives are added in bitumen and bituminous mix, and tested their
viscosity test, penetration values, softening points, ductility test at low temperatures are determined and an
attempt is made to compare the Marshall properties of WMA produced with the chemical additive, Zycotherm
and HMA for Bituminous Concrete (BC) Grade 1. The results of this study showed that the emissions are
significantly reduced during the production and placement of WMA mixtures as compared to the control
HMA mixture. The modified bitumen for warm mix asphalt indicated high consistency and lower
softening point than ordinary bitumen. Warm mix asphalt mixtures also showed better results in term of
strength, stiffness and lower rate of permanent deformation.
Indirect Tensile Strength, Retained Stability, Warm Mix Asphalt, Zycotherm Warm Mix
The asphalt industry all the time looks for a well-organized way to save energy and reducing the emissions.
Rising energy cost and increased environmental awareness due to HMA (Hot Mix Asphalt), Asphalt industry
have brought attention to the potential benefits of Warm Mix Asphalt (WMA) binders. WMA is a fast emerging
new technology with potential of revolutionizing the production of asphalt mix. WMA technology may permit
the mixing, and compaction of asphalt at 30°C to 40°C lower temperatures compared to HMA. WMA is
produced by incorporating additives into asphalt mixtures to let the production and placement of the mix at
temperatures well below the temperatures of conventional HMA.
1.2 Overview of Warm Mix Asphalt (WMA)
It is the generic term for a variety of technologies that allow producers of Hot Mix Asphalt (HMA) pavement
material to lower temperatures at which the material is mixed and placed on the road. It is a proven a technology
260 | P a g ehauled longer distances, Improve working conditions by reducing exposure to fuel emissions, fumes, and odors.
As per the guideline given IRC: SP: 101-2014, the basic principle of this technology is that by adding certain
additives at the final stages of the mix production, the coating of the aggregates by the binder is greatly enhanced
and can be achieved at a considerably less temperature (typically 30°C less) compared to the hot mix process
wherein bitumen is heated to a sufficiently high temperature to make it fluid enough to surround the aggregates
and coat their surfaces.
1.3 Why to Use WMA
The temperatures in cold republics are very low and it is challenging for them to lay the roads in that
temperatures. So they found a new technology for laying the roads at that temperatures. This innovation creates
not only the temperature variance but also evenness to the roads. This creates good looking when compared to
the normal asphalt roads.
It is aimed to propose the optimum dosage of Zycotherm based on laboratory performance evaluation of
bitumen and bituminous mix at different temperature.
To Compare WMA & HMA with or without adding the addmixture.
In this study, bituminous concrete mix has been designed for 19 mm nominal size of aggregate. The aggregate
used in the study is crusher aggregate and VG30 (60/70) grade of Bitumen to check the suitability of aggregates
and bitumen. Firstly, Laboratory testing has been carried out to find the physical properties of aggregates by
conducting tests like aggregate impact value test, crushing value test, Los Angeles abrasion value test, stripping
test, flakiness and elongation index (combined), water absorption and specific gravity Test etc... Similarly, the
Bitumen tests for VG30 have been done including Viscosity test at 60⁰C, Penetration test at 25 °C, Softening
Point test, Ductility test at 27 °C etc. to check the suitability as per IS:73-2013 for both virgin bitumen and
modified bitumen (Zycotherm additives). Thereafter Marshall Mix design method is adopted for HMA and
WMA with different percentage of additives to determine the Optimum bitumen content of bituminous mix at
130⁰C and 115⁰C. After determining the OBC, Marshall Samples are prepared at OBC (130⁰C and 115⁰C) to
check the volumetric properties, Marshall Stability and Flow value as per MORTH 2013 Clause 505.3.1
Specifications. Performance of WMA for BC-1 grade has been evaluated by conducting various tests on
Marshall Samples including Indirect Tensile Strength test, Tensile Strength Ratio and Retained Stability test.
IV. LABORATORY EVALUATION
The aggregates used in this study are crusher aggregates. The sizes of aggregate used are 20 mm, 10mm and
261 | P a g e
Table 1: Physical properties of aggregate
Physical properties of aggregate Test value
4.2 Methods for Finding Properties of Bitumen
4.2.1. Determination of Penetration Value
It measures the hardness or softness of bitumen by measuring the depth in tenths of a millimeter to which a
standard loaded needle will penetrate vertically in 5 seconds. BIS had standardized the equipment and test
procedure. The penetrometer consists of a needle assembly with a total weight of 100g and a device for releasing
and locking in any position. The bitumen is softened to a pouring consistency, stirred thoroughly and poured at a
depth at least 15 mm in excess of the expected penetration. The test should be conducted at a specified
temperature of 25°C. It may be noted that penetration value is largely influenced by any inaccuracy with regards
to pouring temperature, size of the needle, weight placed on the needle and the test temperature.
4.2.2 Ductility test
Ductility is the property of bitumen that permits it to undergo great deformation or elongation. Ductility is
defined as the distance in cm, to which a standard sample or briquette of the material will be elongated without
breaking. Dimension of the briquette thus formed is exactly 1 cm square. The bitumen sample is heated and
poured in the mould assembly placed on a plate. These samples with moulds are cooled in the air and then in
water bath at 27°C temperature. The excess bitumen is cut and the surface is leveled using a hot knife. Then the
mould with assembly containing sample is kept in water bath of the ductility machine for about 90 minutes. The
sides of the moulds are removed, the clips are hooked on the machine and the machine is operated. The distance
up to the point of breaking of thread is the ductility value which is reported in cm. The ductility value gets
affected by factors such as pouring temperature, test temperature, rate of pulling etc.
4.2.3 Softening point test
Softening point denotes the temperature at which the bitumen attains a particular degree of softening under the
specifications of test. The test is conducted by using Ring and Ball apparatus. A brass ring containing test sample
of bitumen is suspended in liquid like water or glycerin at a given temperature. A steel ball is placed upon the
bitumen sample and the liquid medium is heated at a rate of 5°C per minute. Temperature is noted when the
softened bitumen touches the metal plate.
4.2.4 Flash and fire point test
At high temperatures depending upon the grades of bitumen materials leave out volatiles. And these volatiles
catch fire which is very hazardous and therefore it is essential to qualify this temperature for each bitumen grade.
The flash point as the temperature at which the vapour of bitumen momentarily catches fire in the form of flash
under specified test conditions. The fire point is defined as the lowest temperature under specified test conditions
262 | P a g e
4.2.5 Mixing of Zycotherm with Bitumen
The adopted mixing temperatures for HMA was 130°C and 115°C and the mixing temperatures for WMA was
130°C and 115°C, with an additive dosage rate of 0.1%, 0.2%, 0.3% by weight of the binder. The optimum
binder content was to be found out individually for the mixture for different mixing temperatures and additive
V. TENSILE STRENGTH RATIO (TSR) TEST.
Tensile strength ratio is determined according to AASHTO T283, which is the ratio of wet tensile strength to dry
tensile strength of Marshall Specimens. For conditioning of dry samples, Marshall Samples are soaked in water
for 30 minutes at 25°C or are put in air chamber for 4 hours at 25°C. For the conditioning of wet samples, the
samples are placed in water bath for 24 hours at 60°C and then placed in water bath at 25 °C for 2 hours. Then
using Marshall Stability apparatus, Marshall Samples are loaded with compressive load and load at which
specimen fails is measured.
The Tensile Strength Ratio (TSR) is calculated as per below equation
TSR = (Stw/Std)*100
TSR = tensile strength ratio
Stw = average tensile strength of the moisture conditioned subset
Std= average tensile strength of the dry subset
VI. RETAINED MARSHALL STABILITY TEST
This test is conducted as per ASTM D 1075 specifications. Marshall Stability is determined using the standard
procedure i.e. after conditioning the one set of specimen at 60⁰ C for 30-40 minutes. Another set of specimen is
kept for conditioning in water bath maintained at 60°C for 24 hours, and thereafter tested for Marshall Stability
value. The results are reported as the percentage ratio of soak stability to standard stability. This test is conducted
to know that the mix is susceptible to moisture damage or not. The minimum value of Retained Stability of
bituminous mixes is 75% specified by the MORTH section 500 clause 509.
Table 2: Physical properties of Bitumen and Modified Bitumen
Sr. No. Property Test Method Test Results
Requirements as per IS 73:2013 for (Minimum)
1 Absolute viscosity@60°C, Poises IS 1206 (Part 2)-1978 2569.67 2400
2 Penetration,25°C,100 g,5 s, 0.1mm IS 1203-1978 52 45
3 Softening point (R&B),°C IS 1205-1978 50 47
4 Ductility Test, 25°C, cm IS 1208-1978 100 75
5 Absolute viscosity@60°C, Poises IS 1206 (Part 2)-1978 2569.67 2400
263 | P a g e
Property Specified Value
Compaction level 75 blows on either side
Stability, (kN) at 60°C 9 minimum
Flow (mm) 2-4
Marshall Quotient (Stability/Flow) 2-5
Air Voids (%) 3-5
Voids in mineral Aggregate (VMA) (%)
Voids Filled with Bitumen (VFB) (%) 65 – 75 Coating of aggregate particle,
Tensile Strength ratio, minimum 80%
Retained Stability 75 minimum
Table 3 Design requirements for Bituminous Mixes as per MORTH(2013)
Bitumen Test Results
Bitumen Test Test Results Requirement as per IS
73-2013 (Minimum) VG-30 VG-30+Zycotherm mix
0% 0.10% 0.20% 0.30%
Penetration at 25°C 52 52 53 53 45
Softening point (Ring & Ball), °C 50 49 49 48 47
Absolute viscosity@ 60°C, Poises 2569.67 2540 2533 2521.33 2400
Ductility @25 °C ,cm 100+ 100+ 100+ 100+ 75
Table 4 Minimum Percent Voids in Mineral Aggregates (VMA)
Nominal Maximum Particle Size (mm)
Minimum VMA, % Related to Design Air Voids, %
3.0 4.0 5.0
9.5 14.0 15.0 16.0
12.5 13.0 14.0 15.0
19.0 12.0 13.0 14.0
25.0 11.0 12.0 13.0
37.5 10.0 11.0 12.0
VII. RESULTS AND DISCUSSION
The volumetric analysis includes calculation of Bulk density (Gm); Percent Air voids (Vv), Percent Voids in
Mineral Aggregates (VMA), and Percent Voids Filled with Bitumen (VFB). The Mechanical test includes
finding the Marshall Stability and Flow value of Marshall Specimens. This has been carried out for HMA and
WMA at 130⁰C and 115⁰C for all different additives dosage of Zycotherm and at different binder contents. At
each binder content three specimens are made. The average bulk density of three specimens is found out in terms
of gm/cc. The detailed bulk density calculations are shown below. Based on average bulk density, volumetric
analysis is carried out. Correction has to be made for non-standard specimen. So volume calculation for the same
is calculated and Marshall
Stability, Flow calculations for different additive dosage are calculated. Stability and Flow value are taken as
average of three samples to find out Optimum Binder Content (OBC).
The Following figure shows the result of Marshall Stability at 130⁰C &115⁰C for HMA (0%) and WMA (0.1%,
0.2%, and 0.3%) with different additives. The test result is increases first up to 5.5% binder content and then
decreases. The stability of WMA is much better than the stability of HMA , in that the stability of 0.1% additive
is good as compare to other additives.
264 | P a g e
Fig: Stability at 130⁰C
Fig: Stability at 115⁰C
B) Flow at 130⁰C & 115⁰C.
Fig: Flow at 130⁰C Fig: Flow at 115⁰C C) Bulk Density at130⁰C & 115⁰C.
Fig: Bulk Density at 130⁰C Fig: Bulk Density at 115⁰C D) Air Voids at 130⁰C & 115⁰C.
265 | P a g e
E)Voids in mineral aggregates at 130⁰C & 115⁰C.
Fig: Voids in mineral aggregates at 130⁰C Fig: Voids in mineral aggregates at 115⁰C
F) Voids filled with bitumen at 130⁰C & 115⁰C.
Fig: Voids filled with bitumen at 130⁰C Fig: Voids filled with bitumen at 115⁰C
VIII.DETERMINATION OF OPTIMUM BINDER CONTENT (OBC)
Table 5: OBC values for different Zycotherm content
At 130⁰ C At 115⁰ C
Zycotherm contents (%) OBC (%) Zycotherm contents (%) OBC (%)
0 5.35 0 5.18
0.1 5.27 0.1 5.25
0.2 5.22 0.2 5.32
0.3 5.2 0.3 5.2
The Optimum Bitumen Content (OBC) for HMA (0% additive) is 5.35% and 5.18% at 130⁰C and 115⁰C
respectively by weight of mix. The volumetric parameters i.e. Bulk Density, Air Voids, Voids Filled with
Bitumen, Voids in Mineral Aggregates and Marshall Stability and Flow value at Optimum Binder Content
(OBC) are given in Table 6 and Table 7 at 130⁰C and 115⁰C respectively. All parameters satisfies the MORTH
Table 6 : Volumetric Properties at OBC at 130⁰C
Zycotherm content (%) Specified Values as
per MORTH, 2013
0% 0.10% 0.20% 0.30%
Stability (kN) 14.24 15.35 14.01 12.61 > 9
Avg. Flow, (mm) 3.24 3.24 2.84 2.65 2-4
Marshall Quotient 4.05 4.73 4.93 4.77 2-5
Air Voids, % 4.123 4.168 4.208 4.978 3-5
266 | P a g e
Table 7: Volumetric Properties at OBC at 115⁰C
Zycotherm content (%) Specified Values as
per MORTH, 2013
0% 0.10% 0.20% 0.30%
Stability (KN) 12.01 14.35 13.24 13.02 > 9
Avg. Flow, (mm) 2.5 3.12 3.38 2.79 2-4
Marshall Quotient 4.84 4.83 4.17 4.87 2-5
Air Voids, % 4.924 4.729 4.655 4.766 3-5
Voids in Mineral Aggregate, % 16.35 16.39 16.48 16.23 12 minimum Voids Filled with Bitumen, % 69.891 71.143 71.763 70.629 65-75
IX. SUMMARY OF TEST RESULT
The Table No. 8 and Table No. 9 include the summary of test result at OBC with different additive content at
130⁰C and 115⁰C.
Table 8: Summary of test result at 130⁰C
Contents (%) OBC
At OBC (130⁰C)
Gt Gm Vv Vb VMA VFB Bulk Density Stability Flow
0 5.35 2.498 2.395 4.123 12.35 16.473 74.970 2.395 14.24 3.51 0.1 5.27 2.495 2.391 4.168 11.91 16.078 74.075 2.391 15.35 3.24 0.2 5.22 2.495 2.39 4.208 11.62 15.828 73.412 2.39 14.01 2.84 0.3 5.20 2.491 2.367 4.978 11.16 16.138 69.154 2.367 12.61 2.65
Table 9: Summary of test result at 115⁰
Additive Contents (%)
OBC At OBC (115⁰C)
Gt Gm Vv Vb VMA VFB Bulk Density
0 5.18 2.498 2.375 4.924 11.43 16.354 69.891 2.375 12.1 2.5
0.1 5.25 2.495 2.377 4.729 11.66 16.389 71.143 2.377 14.35 3.12 0.2 5.32 2.492 2.376 4.655 11.83 16.485 71.763 2.376 13.24 3.38 0.3 5.20 2.497 2.378 4.766 11.46 16.226 70.629 2.378 13.02 2.79
X. PERFORMANCE EVALUATION OF BITUMINOUS MIXES
Table 10: Retained Stability at 130⁰C
At 130⁰ C (OBC)
Binder Contents (%)
Normal Stability @60⁰ C for 30 minute
Soaked Stability @60⁰ C for 24 hr. Retained Stability (%) MORTH Specification 2013
0 5.35 12.61 11.04 87.55 75 % Minimum
0.1 5.27 14.01 13.02 92.93
0.2 5.22 15.35 14.35 93.49
0.3 5.2 14.35 13.24 92.26
Table 11: Retained Stability at 115⁰C
At 130⁰ C (OBC) Additives (%)
Binder Contents (%)
Normal Stability @60⁰ C for 30 minute
Soaked Stability @60⁰ C for 24 hr.
Retained Stability (%)
MORTH Specification 2013
0 5.18 12.1 10.5 86.78 75 %
0.1 5.25 13.57 12.47 91.89
0.2 5.32 15.06 13.93 92.50
267 | P a g eThe figure I shows the actual representation of how of retained stability are changes as the additives changes
from 0% to 0.3%. The retained stability is increases first and then decreases from 0% to 0.3%. Retained
stability at 115⁰C and 130⁰C having optimum additive content 0.16% and 0.15% respectively.
Fig I: Retained Stability at 130⁰C and 115⁰C
XI. INDIRECT TENSILE STRENGTH TEST
The Dry and Wet Indirect Tensile Strength of Marshall Specimens for HMA and WMA at 130⁰C and 115⁰C,
while Figure II shows the Tensile Strength Ratio (TSR) for the same HMA and WMA at 130⁰C and 115⁰C. The
mixes with 130⁰C showed better TSR than mixes with 115⁰C. This is also understandable as the water
susceptibility of a mix depends the dense mix provides better moisture resistance, as the samples prepared at
130⁰C are more dense than samples at 115⁰C. As per Indian specifications in force, the minimum requirement of
TSR for a bituminous mix is 80 percent and here all mixes pass the test.
Fig II: Tensile Strength Ratio at 130
Based on the detailed study carried out on effect of Zycotherm content for WMA on performance of bitumen and
bituminous mixes, the following conclusions are drawn:
The properties of modified bitumen shown in Table No. 2, satisfies the requirement of Viscosity value, Penetration value, Softening point value and Ductility value as per the Requirement of IS 73-2013.
Bituminous mixes of HMA and WMA prepared by adopting different additive dosage of Zycotherm warm mix additive as mentioned in Table No. 6 and Table No.7 satisfies the requirements of mix given in Table 3.
The values of retained stability and tensile strength ratio of HMA and WMA for given additive contents at 130⁰C and 115⁰C adopted for present study. From Figure: I, it is found that the retained stability at 115⁰C and
130⁰C having optimum additive content 0.16% and 0.15% respectively. And from Figure: II, tensile strength
268 | P a g e
 Kandhal, P.S.(2010). “Warm mix asphalt technologies: An Overview.” Journal of the Indian Roads
Congress, Paper No 561, pp. 143-152.
 Daniel, J. S., and Fowler, J. (2006). “Performance of Warm Mix Asphalt.” New Hampshire Department of
Transportation, New Hampshire.
 Goh, S. W., and You, Z. (2008). “Warm mix asphalt using Sasobit: Field and laboratory experience.” Proc.,
2008 Mid-Continent Transportation Forum, Univ. of Wisconsin, Madison, WI.
 Gandhi, T.S. and Amirkhanian, S.N., (2007), “Laboratory Evaluation of Warm Asphalt Binder Properties –
A Preliminary Analysis”, 5th International Conference of Maintenance and Rehabilitation of Pavements and
Technological Control, Park City.
 Tanveer Khan and Satish Chandra (Department of Civil Engineering, IIT Roorkee (2012). “Effect of warm
mix additives on mixing, laying and compaction temperatures of warm mix binders”.
I S Standard
 IS: 73 (2013), “Paving Bitumen – Specification”, Bureau of Indian Standards, New Delhi.
 IS: 1203 (1978), “Methods for Testing Tar & Bituminous Materials: Determination of Penetration”, Bureau
of Indian Standards, New Delhi.
 IS: 1205 (1978), “Methods for Testing Tar & Bituminous Materials: Determination of Softening Point”,
Bureau of Indian Standards, New Delhi.
 IS: 1208(1978), “Methods for Testing Tar & Bituminous Materials: Determination of Ductility”, Bureau of
Indian Standards, New Delhi.
 IS: 2386 (Part 1) – 1963 (Reaffirmed 2002), “Methods of Test for Aggregates for Concrete – Particle Size
and Shape”, Bureau of Indian Standards, New Delhi.
 IS: 2386 (Part 3) – 1963 (Reaffirmed 2002), “Methods of Test for Aggregates for Concrete – Specific
Gravity, Density, Voids, Absorption and Bulking”, New Delhi.
 IS: 2386 (Part 4) – 1963 (Reaffirmed 2002), “Methods of Test for Aggregates for Concrete – Mechanical
Properties”, Bureau of Indian Standards, New Delhi.
 Ministry of Road Transport and Highways (2013), “Specifications for road and bridge works (Fifth